|Return to index
OSHA Permissible Exposure Limits:
Time Weighted Average............ 0.1 fiber/cc
Excursion Level (30 minutes)..... 1.0 fiber/cc
A known volume of air is drawn through a 25-mm diameter cassette containing a mixed-cellulose ester filter. The cassette must be equipped with an electrically conductive 50-mm extension cowl. The sampling time and rate are chosen to give a fiber density of between 100 to 1,300 fibers/mm2 on the filter.
Recommended Sampling Rate.... 0.5 to 5.0 liters/ minute (L/min)
Recommended Air Volumes:
Minimum...................... 25 L
Maximum...................... 2,400 L
A portion of the sample filter is cleared and prepared for asbestos fiber counting by Phase Contrast Microscopy (PCM) at 400X. Commercial manufacturers and products mentioned in this method are for descriptive use only and do not constitute endorsements by USDOL-OSHA. Similar products from other sources can be substituted.
Chrysotile.............. Mg 3 Si 2 O 5 (OH) 4
Crocidolite............. Na 2 Fe3 2+ Fe 2 3+ Si 8 O 22 (OH) 2
Amosite................. (Mg,Fe) 7 Si 8 O 22 (OH) 2
Tremolite-actinolite.... Ca 2 (Mg,Fe) 7 Si 8 O 22 (OH) 2
Anthophyllite........... (Mg,Fe) 7 Si 8 O 22 (OH) 2
1.3. Advantages and Disadvantages
There are four main advantages of PCM over other methods:
1.4. Workplace Exposure
Asbestos is used by the construction industry in such products as shingles, floor tiles, asbestos cement, roofing felts, insulation and acoustical products. Non-construction uses include brakes, clutch facings, paper, paints, plastics, and fabrics. One of the most significant exposures in the workplace is the removal and encapsulation of asbestos in schools, public buildings, and homes. Many workers have the potential to be exposed to asbestos during these operations.
About 95% of the asbestos in commercial use in the United States is chrysotile. Crocidolite and amosite make up most of the remainder. Anthophyllite and tremolite or actinolite are likely to be encountered as contaminants in various industrial products.
1.5. Physical Properties
Asbestos fiber possesses a high tensile strength along its axis, is chemically inert, non-combustible, and heat resistant. It has a high electrical resistance and good sound absorbing properties. It can be weaved into cables, fabrics or other textiles, and also matted into asbestos papers, felts, or mats.
2. Range and Detection Limit
2.1. The ideal counting range on the filter is 100 to 1,300 fibers/mm 2 With a Walton-Beckett graticule this range is equivalent to 0.8 to 10 fibers/field. Using NIOSH counting statistics, a count of 0.8 fibers/field would give an approximate coefficient of variation (CV) of 0.13.
2.2. The detection limit for this method is 4.0 fibers per 100 fields or 5.5 fibers/mm 2. This was determined using an equation to estimate the maximum CV possible at a specific concentration (95% confidence) and a Lower Control Limit of zero. The CV value was then used to determine a corresponding concentration from historical CV vs. fiber relationships. As an example:
Lower Control Limit (95% Confidence) = AC - 1.645(CV)(AC)
0 = AC - 1.645(CV)(AC)
CV = 0.61
This value was compared with CV vs. count curves. The count at which CV = 0.61 for Leidel-Busch counting statistics or for an OSHA Salt Lake Technical Center (OSHA-SLTC) CV curve (see Appendix A for further information) was 4.4 fibers or 3.9 fibers per 100 fields, respectively. Although a lower detection limit of 4 fibers per 100 fields is supported by the OSHA-SLTC data, both data sets support the 4.5 fibers per 100 fields value.
3. Method Performance - Precision and Accuracy
Precision is dependent upon the total number of fibers counted and the uniformity of the fiber distribution on the filter. A general rule is to count at least 20 and not more than 100 fields. The count is discontinued when 100 fibers are counted, provided that 20 fields have already been counted. Counting more than 100 fibers results in only a small gain in precision. As the total count drops below 10 fibers, an accelerated loss of precision is noted.
At this time, there is no known method to determine the absolute accuracy of the asbestos analysis. Results of samples prepared through the Proficiency Analytical Testing (PAT) Program and analyzed by the OSHA-SLTC showed no significant bias when compared to PAT reference values. The PAT samples were analyzed from 1987 to 1989 (N=36) and the concentration range was from 120 to 1,300 fibers/mm 2.
Fibrous substances, if present, may interfere with asbestos analysis. Some common fibers are:
fiberglass anhydrite plant fibers perlite veins gypsum some synthetic fibers membrane structures sponge spicules diatoms microorganisms wollastonite
The use of electron microscopy or optical tests such as polarized light, and dispersion staining may be used to differentiate these materials from asbestos when necessary.
5.1.1. Sample assembly. Conductive filter holder consisting of a 25-mm diameter, 3-piece cassette having a 50-mm long electrically conductive extension cowl. Backup pad: 25-mm, cellulose. Membrane filter: mixed-cellulose ester (MCE), 25-mm, plain, white, 0.4- to 1.2- m m pore size. Notes:
5.1.2. Gel bands for sealing cassettes.
5.1.3. Sampling pump. Each pump must be a battery operated, self- contained unit small enough to be placed on the monitored employee and not interfere with the work being performed. The pump must be capable of sampling at the collection rate of 2.5 liters per minute (L/min) for the required sampling time.
5.1.4. Flexible tubing, 6 mm bore.
5.1.5. Pump calibration. Stopwatch and bubble tube/burette or electronic meter.
5.2. Sampling Procedure
5.2.1. Seal the point where the base and cowl of each cassette meet with a gel band or tape.
5.2.2. Charge the pumps completely before beginning.
5.2.3. Connect each pump to a calibration cassette with an appropriate length of 6 mm bore plastic tubing. Do not use luer connectors - the type of cassette specified above has built-in adapters.
5.2.4. Select an appropriate flow rate for the situation being monitored. The sampling flow rate must be between 0.5 and 5.0 L/min for personal sampling and is commonly set between 1 and 2 L/min. Always choose a flow rate that will not produce overloaded filters.
5.2.5. Calibrate each sampling pump before and after sampling with a calibration cassette in-line (Note: This calibration cassette should be from the same lot of cassettes used for sampling). Use a primary standard (e.g. bubble burette) to calibrate each pump. If possible, calibrate at the sampling site.
Note: If sampling site calibration is not possible, environmental influences may affect the flow rate. The extent is dependent on the type of pump used. Consult with the pump manufacturer to determine dependence on environmental influences. If the pump is affected by temperature and pressure changes, correct the flow rate using the formula shown in the section "Sampling Pump Flow Rate Corrections" at the end of this appendix.
5.2.6. Connect each pump to the base of each sampling cassette with flexible tubing. Remove the end cap of each cassette and take each air sample open face. Assure that each sample cassette is held open side down in the employee's breathing zone during sampling. The distance from the nose/mouth of the employee to the cassette should be about 10 cm. Secure the cassette on the collar or lapel of the employee using spring clips or other similar devices.
5.2.7. A suggested minimum air volume when sampling to determine TWA compliance is 25 L. For Excursion Limit (30 min sampling time) evaluations, a minimum air volume of 48 L is recommended.
5.2.8. The most significant problem when sampling for asbestos is overloading the filter with non-asbestos dust. Suggested maximum air sample volumes for specific environments are:
Environment Air Vol. (L)
Asbestos removal operations (visible dust) 100
Asbestos removal operations (little dust) 240
Office environments. 400 to 2,400
CAUTION: Do not overload the filter with dust. High levels of non- fibrous dust particles may obscure fibers on the filter and lower the count or make counting impossible. If more than about 25 to 30% of the field area is obscured with dust, the result may be biased low. Smaller air volumes may be necessary when there is excessive non-asbestos dust in the air.
While sampling, observe the filter with a small flashlight. If there is a visible layer of dust on the filter, stop sampling, remove and seal the cassette, and replace with a new sampling assembly. The total dust loading should not exceed 1 mg.
5.2.9. Blank samples are used to determine if any contamination has occurred during sample handling. Prepare two blanks for the first 1 to 20 samples. For sets containing greater than 20 samples, prepare blanks as 10% of the samples. Handle blank samples in the same manner as air samples with one exception: Do not draw any air through the blank samples. Open the blank cassette in the place where the sample cassettes are mounted on the employee. Hold it open for about 30 seconds. Close and seal the cassette appropriately. Store blanks for shipment with the sample cassettes.
5.2.10. Immediately after sampling, close and seal each cassette with the base and plastic plugs. Do not touch or puncture the filter membrane as this will invalidate the analysis.
5.2.11. Attach and secure a sample seal around each sample cassette in such a way as to assure that the end cap and base plugs cannot be removed without destroying the seal. Tape the ends of the seal together since the seal is not long enough to be wrapped end-to-end. Also wrap tape around the cassette at each joint to keep the seal secure.
5.3. Sample Shipment
5.3.1. Send the samples to the laboratory with paperwork requesting asbestos analysis. List any known fibrous interferences present during sampling on the paperwork. Also, note the workplace operation(s) sampled.
5.3.2. Secure and handle the samples in such that they will not rattle during shipment nor be exposed to static electricity. Do not ship samples in expanded polystyrene peanuts, vermiculite, paper shreds, or excelsior. Tape sample cassettes to sheet bubbles and place in a container that will cushion the samples in such a manner that they will not rattle.
5.3.3. To avoid the possibility of sample contamination, always ship bulk samples in separate mailing containers.
6.1.1. Acetone is extremely flammable and precautions must be taken not to ignite it. Avoid using large containers or quantities of acetone. Transfer the solvent in a ventilated laboratory hood. Do not use acetone near any open flame. For generation of acetone vapor, use a spark free heat source.
6.1.2. Any asbestos spills should be cleaned up immediately to prevent dispersal of fibers. Prudence should be exercised to avoid contamination of laboratory facilities or exposure of personnel to asbestos. Asbestos spills should be cleaned up with wet methods and/or a High Efficiency Particulate Air (HEPA) filtered vacuum.
CAUTION: Do not use a vacuum without a HEPA filter - It will disperse fine asbestos fibers in the air.
6.2.1. Phase contrast microscope with binocular or trinocular head.
6.2.2. Widefield or Huygenian 10X eyepieces (NOTE: The eyepiece containing the graticule must be a focusing eyepiece. Use a 40X phase objective with a numerical aperture of 0.65 to 0.75).
6.2.3. Kohler illumination (if possible) with green or blue filter.
6.2.4. Walton-Beckett Graticule, type G-22 with 100 plus or minus 2 m m projected diameter.
6.2.5. Mechanical stage. A rotating mechanical stage is convenient for use with polarized light.
6.2.6. Phase telescope.
6.2.7. Stage micrometer with 0.01-mm subdivisions.
6.2.8. Phase-shift test slide, mark II (Available from PTR optics Ltd., and also McCrone).
6.2.9. Precleaned glass slides, 25 mm X 75 mm. One end can be frosted for convenience in writing sample numbers, etc., or paste-on labels can be used.
6.2.10. Cover glass #1 1/2.
6.2.11. Scalpel (#10, curved blade).
6.2.12. Fine tipped forceps.
6.2.13. Aluminum block for clearing filter (see Appendix D and Figure 4).
6.2.14. Automatic adjustable pipette, 100-to 500- m L.
6.2.15. Micropipette, 5 m L.
6.3.1. Acetone (HPLC grade).
6.3.2. Triacetin (glycerol triacetate).
6.3.3. Lacquer or nail polish.
6.4. Standard Preparation
6.5. Sample Mounting
Note: See Safety Precautions in Section 6.1. before proceeding. The objective is to produce samples with a smooth (non-grainy) background in a medium with a refractive index of approximately 1.46. The technique below collapses the filter for easier focusing and produces permanent mounts which are useful for quality control and interlaboratory comparison.
An aluminum block or similar device is required for sample preparation.
6.5.1. Heat the aluminum block to about 70 deg.C. The hot block should not be used on any surface that can be damaged by either the heat or from exposure to acetone.
6.5.2. Ensure that the glass slides and cover glasses are free of dust and fibers.
6.5.3. Remove the top plug to prevent a vacuum when the cassette is opened. Clean the outside of the cassette if necessary. Cut the seal and/or tape on the cassette with a razor blade. Very carefully separate the base from the extension cowl, leaving the filter and backup pad in the base.
6.5.4. With a rocking motion cut a triangular wedge from the filter using the scalpel. This wedge should be one-sixth to one-fourth of the filter. Grasp the filter wedge with the forceps on the perimeter of the filter which was clamped between the cassette pieces. DO NOT TOUCH the filter with your finger. Place the filter on the glass slide sample side up. Static electricity will usually keep the filter on the slide until it is cleared.
6.5.5. Place the tip of the micropipette containing about 200 m L acetone into the aluminum block. Insert the glass slide into the receiving slot in the aluminum block. Inject the acetone into the block with slow, steady pressure on the plunger while holding the pipette firmly in place. Wait 3 to 5 seconds for the filter to clear, then remove the pipette and slide from the aluminum block.
6.5.6. Immediately (less than 30 seconds) place 2.5 to 3.5 m L of triacetin on the filter (NOTE: Waiting longer than 30 seconds will result in increased index of refraction and decreased contrast between the fibers and the preparation. This may also lead to separation of the cover slip from the slide).
6.5.7. Lower a cover slip gently onto the filter at a slight angle to reduce the possibility of forming air bubbles. If more than 30 seconds have elapsed between acetone exposure and triacetin application, glue the edges of the cover slip to the slide with lacquer or nail polish.
6.5.8. If clearing is slow, warm the slide for 15 min on a hot plate having a surface temperature of about 50 deg.C to hasten clearing. The top of the hot block can be used if the slide is not heated too long.
6.5.9. Counting may proceed immediately after clearing and mounting are completed.
6.6. Sample Analysis
Completely align the microscope according to the manufacturer's instructions. Then, align the microscope using the following general alignment routine at the beginning of every counting session and more often if necessary.
6.6.2. Counting Fibers
6.7. Fiber Identification
As previously mentioned in Section 1.3., PCM does not provide positive confirmation of asbestos fibers. Alternate differential counting techniques should be used if discrimination is desirable. Differential counting may include primary discrimination based on morphology, polarized light analysis of fibers, or modification of PCM data by Scanning Electron or Transmission Electron Microscopy.
6.8. Analytical Recommendations - Quality Control System
6.8.1. All individuals performing asbestos analysis must have taken the NIOSH course for sampling and evaluating airborne asbestos or an equivalent course.
6.8.2. Each laboratory engaged in asbestos counting shall set up a slide trading arrangement with at least two other laboratories in order to compare performance and eliminate inbreeding of error. The slide exchange occurs at least semiannually. The round robin results shall be posted where all analysts can view individual analyst's results.
6.8.3. Each laboratory engaged in asbestos counting shall participate in the Proficiency Analytical Testing Program, the Asbestos Analyst Registry or equivalent.
6.8.4. Each analyst shall select and count prepared slides from a "slide bank". These are quality assurance counts. The slide bank shall be prepared using uniformly distributed samples taken from the workload. Fiber densities should cover the entire range routinely analyzed by the laboratory. These slides are counted blind by all counters to establish an original standard deviation. This historical distribution is compared with the quality assurance counts. A counter must have 95% of all quality control samples counted within three standard deviations of the historical mean. This count is then integrated into a new historical mean and standard deviation for the slide.
The analyses done by the counters to establish the slide bank may be used for an interim quality control program if the data are treated in a proper statistical fashion.
7.1. Calculate the estimated airborne asbestos fiber concentration on the filter sample using the following formula:
Image 1 (0.5" X 1.75") Not available for Offline Print to STP or FAX
7.2. Short-Cut Calculation
Since a given analyst always has the same interpupillary distance, the number of fields per filter for a particular analyst will remain constant for a given size filter. The field size for that analyst is constant (i.e. the analyst is using an assigned microscope and is not changing the reticle).
For example, if the exposed area of the filter is always 385 mm 2 and the size of the field is always 0.00785 mm 2 the number of fields per filter will always be 49,000. In addition it is necessary to convert liters of air to cc. These three constants can then be combined such that ECA/(1,000 x MFA)=49. The previous equation simplifies to:
Image 2 (0.5" X 1.5") Not available for Offline Print to STP or FAX
7.3. Recount Calculations
As mentioned in step 13 of Section 6.6.2., a "blind recount" of 10% of the slides is performed. In all cases, differences will be observed between the first and second counts of the same filter wedge. Most of these differences will be due to chance alone, that is, due to the random variability (precision) of the count method. Statistical recount criteria enables one to decide whether observed differences can be explained due to chance alone or are probably due to systematic differences between analysts, microscopes, or other biasing factors.
The following recount criterion is for a pair of counts that estimate AC in fibers/cc. The criterion is given at the type-I error level. That is, there is 5% maximum risk that we will reject a pair of counts for the reason that one might be biased, when the large observed difference is really due to chance.
Reject a pair of counts if:
Image 3 (0.25" X 2.5") Not available for Offline Print to STP or FAX
7.4. Reporting Results
Report results to the industrial hygienist as fibers/cc. Use two significant figures. If multiple analyses are performed on a sample, an average of the results is to be reported unless any of the results can be rejected for cause.
8.1. Dreesen, W.C., et al., U.S. Public Health Service: A Study of Asbestosis in the Asbestos Textile Industry (Public Health Bulletin No. 241), U.S. Treasury Dept., Washington, DC, 1938.
8.2. Asbestos Research Council: The Measurement of Airborne Asbestos Dust by the Membrane Filter Method (Technical Note), Asbestos Research Council, Rockdale, Lancashire, Great Britain, 1969.
8.3. Bayer, S.G., Zumwalde, R.D., Brown, T.A., Equipment and Procedure for Mounting Millipore Filters and Counting Asbestos Fibers by Phase Contrast Microscopy, Bureau of Occupational Health, U.S. Dept. of Health, Education and Welfare, Cincinnati, OH, 1969.
8.4. NIOSH Manual of Analytical Methods, 2nd ed., Vol. 1 (DHEW/ NIOSH Pub. No. 77-157-A). National Institute for Occupational Safety and Health, Cincinnati, OH, 1977. pp. 239-1 - 239-21.
8.5. Asbestos, Code of Federal Regulations 29 CFR 1910.1001. 1971.
8.6. Occupational Exposure to Asbestos, Tremolite, Anthophyllite, and Actinolite. Final Rule, Federal Register 51:119 (20 June 1986). pp. 22612- 22790.
8.7. Asbestos, Tremolite, Anthophyllite, and Actinolite, Code of Federal Regulations 1910.1001. 1988. pp. 711-752.
8.8. Criteria for a Recommended Standard - Occupational Exposure to Asbestos (DHEW/NIOSH Pub. No. HSM 72-10267), National Institute for Occupational Safety and Health, NIOSH, Cincinnati, OH, 1972. pp. III-1 - III-24.
8.9. Leidel, N.A., Bayer, S.G., Zumwalde, R.D., Busch, K.A., USPHS/NIOSH Membrane Filter Method for Evaluating Airborne Asbestos Fibers (DHEW/NIOSH Pub. No. 79-127). National Institute for Occupational Safety and Health, Cincinnati, OH, 1979.
8.10. Dixon, W.C., Applications of Optical Microscopy in Analysis of Asbestos and Quartz, Analytical Techniques in Occupational Health Chemistry, edited by D.D. Dollberg and A.W. Verstuyft. Wash. D.C.: American Chemical Society, (ACS Symposium Series 120) 1980. pp. 13-41.
The OSHA asbestos regulations require each laboratory to establish a quality control program. The following is presented as an example of how the OSHA-SLTC constructed its internal CV curve as part of meeting this requirement. Data is from 395 samples collected during OSHA compliance inspections and analyzed from October 1980 through April 1986.
Each sample was counted by 2 to 5 different counters independently of one another. The standard deviation and the CV statistic was calculated for each sample. This data was then plotted on a graph of CV vs. fibers/mm 2. A least squares regression was performed using the following equation:
CV = antilog 10 [A(log 10 (x)) 2 +B(log 10 (x))+C]
x = the number of fibers/mm 2
Application of least squares gave:
Image 4 (0.5" X 2") Not available for Offline Print to STP or FAX
2.93 x 100
d c = ___________ =2.71mm
Image 5 (0.5" X 1") Not available for Offline Print to STP or FAX
Image 6 (6.5" X 7") Not available for Offline Print to STP or FAX
Structure No. Count Explanation
1 to 6 1 Single fibers all contained within the Circle.
7 1/2 Fiber crosses circle once.
8 0 Fiber too short.
9 2 Two crossing fibers.
10 0 Fiber outside graticule.
11 0 Fiber crosses graticule twice.
12 1/2 Although split, fiber only crosses once.
Government Code section 11346.2(d) (Register 91, No. 19).
2. Editorial correction of HISTORY 1 (Register 91, No. 45).
3. Editorial correction of Appendix B (Register 95, No. 41).
4. Repealer and new appendix and Note filed 5-3-96; operative 7-3-96 (Register
96, No. 18).
5. Change without regulatory effect providing more legible Figure 1 filed 1-20-
2008 pursuant to section 100, title 1, California Code of Regulations
(Register 2009, No. 4).